Correlations Between Molecular Architecture, Morphology and
Deformation Behaviour of Styrene/Butadiene
Block Copolymers and Blends
zur Erlangung des Akademischen Grades
Mathematisch-Naturwissenschaftlich-Technischen Fakultät (Ingenieurwissenschaftlicher Bereich)
der Martin-Luther-Universität Halle-Wittenberg
von Herrn M. Sc. Chem. Rameshwar Adhikari geb. am 03.09.1963 in Nuwakot/Nepal
1. Prof. Dr. rer. nat. G. H. Michler 2. Prof. Dr. F. J. Baltá Calleja 3. Prof. Dr.-Ing. V. Altstädt
Merseburg, den 30.11.2001 urn:nbn:de:gbv:3-000003100
For many helpful suggestions, discussions, supports and inspirations; and providing me an opportunity to work in his prosperous group ‘Morphologie und Mikromechanik’ and write this thesis on one of the most fascinating scientific topics of nanostructured polymeric materials under his intensive guidance, I sincerely extend my thanks to Prof. G.H. Michler.
Many sincere thanks go to Dr. R. Godehardt for teaching me AFM techniques, for his fatherly support in every respects and helps during the clarification of several bureaucratic issues. Thanks are due to W. Lebek for his untiring helps in many aspects like software, computer problematic, AFM experiments etc.
I would like to thank S. Goerlitz (TEM), C. Becker and S. Henning (SEM) and Dr. E. Ivankova (HVEM) for beautiful electron micrographs which form the soul of this thesis. Many thanks are due to C. Hatscher for helping design many nice schemes. Dr. T.A. Huy is thanked for carrying out DMA as well as DSC experiments. Many helpful discussions, suggestions and helps from Dr. R. Weidisch are acknowledged. Special thanks go to Dr. R. Lach for many scientific discussions and helps in fracture mechanics investigations. Intensive helps from C. Becker, S. Goerlitz, S. Henning, J. Laatsch and V. Seydewitz are simply unforgettable.
I extend my sincere thanks to Doz. Dr. K. Schmutzler, C. Wittig, E. Kühnberger and H. Otto for their co-operation. Diverse helps from groups of Prof. Grellmann, Prof. Kreßler, Prof. Radusch, Prof. Arnold and Doz. Dr. Höring are earnestly acknowledged. Co-operation with P. Simon (Dresden), M. Buschnakowski, M. Schoßig, S. Dunger and S. Großstück are hearty acknowledged.
I would like to acknowledge the BASF AG, especially Dr. K. Knoll, for the fruitful co-operation and providing the samples and characterisation data. Co-operation with Dr. K. Geiger (Universität Stuttgart) and M. Langela (MPI-P, Mainz) in the frame of the BASF-Project-‘Styrol/Butadien-Blockcopolymere’ is sincerely acknowledged. I am indebted to the Land Sachsen-Anhalt and the Max-Buchner-Forschungsstiftung for financial support.
I am greatly indebted to the members of our group for their warm affection. Everyday before I started to work (often during coffee hour), the people around the table (whom I feel as my family) frequently asked me if I need help; if I have any kinds of troubles; whether my family is ok etc.; and they helped me from the depth of their hearts. These were the most important things that always inspired me and enhanced my works. I would like to thank once again the whole group for this family environment. I thank my wife Pooja for her unlimited patient and moral support; it would have been impossible to successfully terminate this mission without her understanding and help. Finally, I acknowledge the efforts of my parents to make me able stand on my foot; and dedicate this work to my children
PariPurak who think that polymers are the things to play with.
Warm reception from many Merseburger and Hallenser have also contributed indirectly to make our stay in Germany a pleasant experience and make this work a success.
1. INTRODUCTION 1
1.1 Significance of Block Copolymers 1
1.2 Aims and Overview of Thesis 2
1.3 Sample Preparation and Investigation Methods 3
2. STRUCTURE-PROPERTY-CORRELATIONS OF BLOCK COPOLYMERS 4
2.1 Microphase Separation and Morphology 4
2.2 Morphology Control via Architectural Modification 9
2.2.1 Variation of Chain Topology 9
2.2.2 Asymmetric Block Structure 12
2.2.3 Interfacial Modification 14
2.3 Blends Containing Block Copolymers 16
2.3.1 Block Copolymer/Homopolymer Blends 16
2.3.2 Binary Block Copolymer Blends 19
2.4 Mechanical Properties and Deformation Behaviour 21
2.4.1 Thermomechanical Properties 21
2.4.2 Mechanical Behaviour of Polymers 22
2.4.3 Micromechanical Construction of Polymers 24
2.4.4 Deformation Behaviour of Styrenic Block Copolymers 26
2.4.5 Molecular Architecture vs. Micromechanics 37
3. EXPERIMENTAL PART 39
3.1 Materials 39
3.1.1 Pure Block Copolymers 39
3.1.2 Block Copolymer/Hompolystyrene (hPS) Blends 39
3.1.3 Binary Block Copolymer Blends 39
3.1.4 Synthesis of Block Copolymers 39
3.2 Sample Preparation 42 3.3 Mechanical Properties 42 3.3.1 Tensile Testing 43 3.3.2 Fracture Mechanics 43 3.4 Microscopic Techniques 45 3.4.1 Electron Microscopy 45
3.4.2 Scanning Force Microscopy 46
3.5.1 Thermomechanical Properties and Glass Transitions 46
3.5.2 Molecular Weight and Composition 46
4. STRUCTURE-PROPERTY-CORRELATIONS IN DIFFERENT BLOCK
COPOLYMER ARCHITECTURES 47
4.1 Phase Behaviour and Morphology 47
4.1.1 Correlation Between Molecular Architecture and Phase Behaviour 47
4.1.2 Equilibrium Morphologies 50
4.1.3 Effects of Sample Preparation Methods 57
4.2 Mechanical Properties 59
4.2.1 Tensile Behaviour 59
4.2.2 Mechanical Anisotropy in Oriented Samples 62
4.3 Micromechanical Behaviour 63
4.3.1 Influence of Microphase Morphology 63
4.3.2 Influence of Molecular Structure 70
4.3.3 Thin Layer Yielding Mechanism in Lamellar Star Block Copolymers 74
4.3.4 Additional Evidences of Thin Layer Yielding Mechanism 78
4.4 Fracture Toughness of the Block Copolymers 80
4.5 Conclusions 82
5. STRUCTURE-PROPERTY-CORRELATIONS IN BLOCK COPOLYMER/PS
5.1 Phase Behaviour and Morphology 84
5.1.1 Dynamic Mechanical Properties 84
5.1.2 Influence of hPS Molecular Weight on Morphology 85
5.1.3 Morphology of Injection Moulds 88
5.2 Mechanical Properties 92
5.2.1 Tensile Behaviour 92
5.2.2 Fracture Mechanics 95
5.3 Micromechanical Deformation Behaviour 97
5.3.1 Solution Cast Blends 97
5.3.2 Injection Moulded Blends 102
6. STRUCTURE-PROPERTY-CORRELATIONS IN BINARY BLOCK COPOLYMER
6.1 Motivation – Why Binary Block Copolymer Blends? 110
6.2 Phase Behaviour and Morphology 111
6.2.1 Phase Behaviour and Equilibrium Morphologies 111
6.2.2 Morphology of Injection Moulded Samples 116
6.3 Mechanical Properties and Micromechanical Behaviour 117
6.3.1 Tensile Properties 117
6.3.2 Toughness Characterisation by Fracture Mechanics Approach 121
6.4 Conclusions 128
7. SUMMARY AND PERSPECTIVES 130
8. ZUSAMMENFASSUNG UND PERSPEKTIVE 134
9. REFERENCES 139
LIST OF ABBREVIATIONS AND SYMBOLS
a distance between two adjacent chemical junctions along an interface/statistical segment length (Kuhn length)
a/a0 relative distance between the adjacent chemical junction points
∆a stable crack growth
α degree of polymerisation of homopolystyrene relative to that of corresponding block of the block copolymer (NhPS/ NPS-block)
bcc body centred cubic
sec-BuLi secondary butyllithium
CTOD crack tip opening displacement (δ) χ Flory-Huggins interaction parameter D domain thickness
Dcrit critical thickness of lamellae
DG double gyroid
DMA dynamic mechanical analysis DSC differential scanning calorimetry EB etylene/butylene copolymer
Ed Young’s modulus determined in impact test
ESIS TC4 European structural integrity society, technical committee 4: polymers and composites
ε strain, (also mol. Asymmetry parameter used by Milner, ref. )
F impact load
f composition of block copolymer (also represented by Φ)/deflection of the specimen during impact testing
fc composition of block copolymer at which the continuous transition from disordered
to lamellar phase occurs
FTIR Fourier transform infra-red spectroscopy G′ dynamic storage shear modulus
G′′ dynamic loss modulus
GPC gel permeation chromatography ∆G Gibbs’s free energy
hex hexagonal phase (also hpc) HML hexagonal modulated layers hpc hexagonal packed cylinders HPL hexagonal perforated lamellae hPS polystyrene homopolymer
HVEM high voltage electron microscope ∆H enthalpy change
ISR intermediate segregation regime
J0.1 J-integral value determined at a stable crack growth of 0.1 mm at the point of
technical crack initiation
Ji J-integral value as resistance against stable crack initiation called physical crack
JId J-integral value as resistance against unstable crack initiation for crack opening mode
I, geometry independent parameter k Boltzmann’s constant
L long period of domains lam lamellar phase
λ extension ratio, λmax maximum extension ratio
MEK methyl ethyl ketone
MSS microphase separated structures
Mw weight average molecular weight
N total degree of polymerisation
NhPS degree of polymerisation of polystyrene homopolymer
NPS-block degree of polymerisation of polystyrene block of a block copolymer
OBDD ordered bicontinuous double diamond ODT order-disorder transition
OOT order-order transition OsO4 osmium tetroxide
PB polybutadiene PE polyethylene PEO polyethylene oxide PI polyisoprene
PMMA polymethyl methaacrylate P2VP polyvinyl pyridine
PP polypropylene PPO polyphenylene oxide PS polystyrene
PVC polyvinyl chloride R-curves crack resistance curves R g radius of gyration
SAXS small angle X-ray scattering
SB block copolymer consisting of polystyrene and polybutadiene
S/B a statistical copolymer of styrene and butadiene (styrene-co-butadiene) SBS styrene-b-butadiene-b-styrene triblock copolymer
SBR styrene/butadiene rubber SCFT self consistent field theory SEM scanning electron microscopy SFM scanning force microscopy
SIS styrene-b-isoprene-b-styrene triblock copolymer SSL strong segregation limit
∆S entropy change
σy yield stress
σYlam yield stress of PS lamellae
tanδ dynamic loss tangent (G’’/G’) TEM transmission electron microscopy Tg glass transition temperature
TPE thermoplastic elastomer
τ asymmetry parameter as introduced by de la Cruz, ref.  WSL weak segregation limit
1. INTRODUCTION 1.1 Significance of Block Copolymers
Polymeric materials offer a wide range of application relevant properties. Therefore, these materials find growing applications in various fields of everyday life. Since their ultimate properties are determined by their chemical microstructures, control of chemical structure (macromolecular designing) is the first step of creating materials of desired properties profile. In practice, different properties are simultaneously desirable, e.g. a combination of stiffness and drawability, or strength and toughness etc. A technological way of achieving these combinations is the heterogenisation of existing polymers. Polymer blends represent this strategy of designing polymeric materials [1-3].
Blending may often lead to the deterioration of the mechanical properties due to insufficient phase adhesion resulting from the incompatibility of the blend components; hence these blends need compatibilisation. One of the strategy being practiced for about 50 years to get rid of this problem is to join the desired polymer chains with a primary covalent bond which has given rise to today’s fascinating world of block copolymers [2-4].
All block copolymers belong to a broad category of condensed matter sometimes referred collectively as soft materials, which, in contrast to crystalline solids, are characterised by fluid-like disorder on the molecular scale and a high degree of order at longer length scales. Combining the incompatible polymer chains in a single macromolecule leads to intra-molecular phase separation whereby the problem of inadequate phase adhesion will be eliminated. This, in turn, leads to the formation of highly ordered self-assembled “crystalline-like” phase separated structures in melt as well as solid state whose periodicity lies in the range of radius of gyration (Rg) of the constituent molecules. The nature and size of these structures can be controlled by
various methods including interfacial and architectural modification .
The block copolymers find application in diverse fields: as thermoplastic elastomers, pressure sensitive adhesives, impact modifiers, compatibilisers etc. In solutions, their surfactant properties are exploited in foams, oil additives, solubilisers, thickeners and dispersion agents. The block copolymers may have potential applications in medicines, nanotempleting and nanotechnology . An annual growth rate of 9-10% of thermoplastic elastomers (compared to 2-4% growth rate of other polymers) in the last 20 years reflects the significance of these materials in polymer market .
Recently, synthesis of several block copolymer architectures including ABC triblock copolymers has triggered the discovery of novel morphologies and opened new potential of controlling mechanical properties . Especially, the block copolymers with complex molecular characteristics are being paid special attention.
1.2 Aims and Overview of Thesis
Styrene/butadiene block copolymers find applications as thermoplastic elastomers, moulding products, toughness modifiers and films. They are, generally, not used commercially as pure materials but compounded with other polymers, fillers etc. to achieve the particular requirements for each end-use. In many applications, mechanical properties are of prime interest. In spite of a detailed knowledge of phase behaviour of simple linear block copolymers, correlation between their morphology, mechanical properties and micromechanical mechanisms, very important for technical applications, is not well understood. Hence, it is of prime importance from materials scientific stand point that this correlation is intensively investigated.
The primary goal of this work is to investigate experimentally correlations between phase behaviour, morphology and micromechanical deformation behaviour of block copolymers (and blends) as a function of their molecular architecture.
The work is limited to amorphous styrene/butadiene block copolymers in a narrow composition range (Φstyrene ~ 0.70) with an special emphasis on few selected asymmetric architectures.
Detailed discussion of morphology development in a wide composition range and their synthetic and rheological aspects are outside the scope of this thesis. The thesis has been organised in the following way:
A short review of thermodynamics, morphology and deformation behaviour of amorphous block copolymers is given in chapter 2. Chapter 3 deals with experimental techniques and general methods of synthesising block copolymers of the types used in this study. Experimental results are discussed in chapters 4, 5 and 6. A brief summary of the research works and future perspective are given in chapter 7.
First, influence of block copolymer architecture on microphase morphology and ultimate mechanical properties of styrene/butadiene block copolymers, which is the main issue of this work, is discussed in chapter 4. For this purpose, phase behaviour, morphology, mechanical properties and micromechanical deformation mechanisms of linear and star shaped block copolymers having different interfacial structures are comparatively analysed.
Styrene/butadiene block copolymers are often used in combination with polystyrene homopolymer (hPS) which find applications in injection moulded parts, food packaging films and beakers for soft and warm drinks. In such applications, a balance between transparency and toughness lies in the centre of interest. Hence, another objective is to study the morphology and micromechanical as well as mechanical behaviour of binary star block copolymer/hPS blends in chapter 5.
Finally, binary block copolymer blends offer new possibilities of tailoring mechanical properties. Despite a few works on phase behaviour and morphology of block copolymer blends, no systematic works about their mechanical behaviour are reported. Structure-property correlations of binary block copolymer blends (star block and triblock) shall be discussed in chapter 6 especially using several concepts of elastic-plastic fracture mechanics.
1.3 Sample Preparation and Investigation Methods
Block copolymers samples synthesised via living anionic polymerisation and provided by the BASF were prepared by different methods: solution casting, extrusion, injection and compression moulding. Polystyrene homopolymers used to blend with selected block copolymers were synthesised by radical polymerisation.
Electron microscopy (TEM, SEM and HVEM) and scanning force microscopy (SFM) were used as principal experimental tools. Mechanical properties are characterised by tensile and impact testing. Dynamic mechanical analysis (DMA) and differential scanning calorimetry (DSC) were employed to determine the glass transition temperature and gain insight into the phase behaviour of the materials. Samples were prepared by solution casting and common processing techniques (injection moulding, press moulding and extrusion).
2. STRUCTURE-PROPERTY-CORRELATIONS OF BLOCK COPOLYMERS
2.1 Microphase Separation and Morphology
If two polymers are mixed, the most frequent result is a system that exhibits a complete phase separation due to the repulsive interaction between the components (i.e. the chemical incompatibility between the polymers) [6-8]. Complete miscibility in a mixture of two polymers requires that the following conditions be fulfilled.
0 < ∆ − ∆ = ∆Gm Hm T Sm i.e., ∆Gm =-ve, (2.1)
where ∆Gm, ∆Hm, and ∆Sm stand for Gibb´s free energy, enthalpy and entropy of mixing at
temperature T, respectively. Generally, ∆Hm and T∆Sm are both positive for polymer pairs. The
value of T∆Sm is always positive since there is an increase in the entropy on mixing. Therefore
the sign of ∆Gm always depends on the value of the enthalpy of mixing ∆Hm. Surprisingly the
heat of mixing is usually positive which does not favour mixing. Hence, the polymer pairs mix to form a single phase only if the entropic contribution to free energy exceeds enthalpic contribution, i.e.,
m T S
H < ∆
The lattice theory for the enthalpy of mixing in polymer solutions, developed by Flory and Huggins, can be formally applied to polymer mixtures, which provides a rough estimation of the miscibility of the polymers. The entropy and enthalpy of mixing of two polymers are given by [7,8]:
[1 lnΦ1 + 2lnΦ2
]− = ∆Sm k n n (2.3) 2 1 12 Φ Φ = ∆Hm kTχ N (2.4)
where φi is the volume fraction of the polymer i and N = n1 + n2 is the total number of polymer
molecules in the mixture. χ is called Flory-Huggin’s interaction parameter. Hence, enthalpic and entropic contribution to free energy of mixing can be parameterised in terms of Flory-Huggins segmental interaction parameter χ and the degree of polymerisation N, respectively.
The fundamental thermodynamics of phase separation in polymer blends is applicable to block copolymers as well. The phase behaviour of a bulk two-component block copolymer AB is determined by three experimentally controllable factors [2,4,9-11]:
i. the overall degree of polymerisation N,
ii. architectural constrains (diblock, triblock, star block etc.) and composition f (overall volume fraction of component A),
The first two factors are regulated through the polymerisation stoichiometry and affect the translational and configurational entropy, while the magnitude of (the largely enthalpic) χ is determined by selection of A-B monomer pairs, and has a temperature dependence given by:
where α and β are constant depending on composition and architectural constrains of the block copolymer.
At equilibrium, the block copolymer chains assume the lowest free energy configuration. Increasing the energy parameter χ ( i.e., lowering the temperature) favours a reduction in A-B monomer contacts. If the value of N is sufficiently large, it is accomplished with some loss of translational and configurational entropy by local compositional ordering . Such local segregation is referred to as microphase separation in the block copolymer. Alternatively, if χ or N is decreased enough, the entropic factor will dominate, leading to a compositionally disordered phase. Since the entropic and enthalpic contribution to free energy density scale respectively as N-1 and χ, it is the product χN that dictates the block copolymer phase state, and it is called the reduced interaction parameter or lumped interaction parameter [9-11]. When the value of this parameter exceeds a certain value specific for the system under consideration, the microphase-separated structures evolve below which the system is in the disordered state. This phenomenon is called microphase separation transition (MST) or order-disorder transition (ODT) . For a symmetric diblock copolymer (i.e., composition f = 0.5) the transition occurs when χN ≈ 10.5 [10-14]. At sufficiently large values of χN, different ordered structures are formed in the melt as well as in the solid state. These structures, also termed as microphase separated structures (MSS), are best represented in the form of phase diagrams (Appendix 2.1) which are generally constructed by plotting the lumped parameter (χN) as a function of composition. Two limiting regimes have been postulated in the block copolymer phase diagrams, as illustrated in figure 2.1. For χN<<1, a copolymer melt is disordered and the A-B interaction is sufficiently low that the individual chains assume unperturbed Gaussian statistics. The composition profile is almost sinusoidal (fig 2.1a), and the domain periodicity L scales as :
2 / 1 aN R L∝ g ∝ , (2.6)
where a is the characteristic segment length; Rg and N stand for gyration radius of copolymer
molecule and polymerisation index, respectively.
This regime is called weak segregation limit and the copolymers showing this behaviour are characterised by a widened interface due to enhanced phase mixing. Approaching this regime, thermotropic order-order transitions are predicted. A thermoreversible morphology transition at the upper portion of the phase diagrams is allowed.
As the value of χN is greater than 10, nearly pure A and B domains are formed. The chain conformation is, in this case, no longer Gaussian one but rather perturbed (stretched chain conformation). This regime is termed as strong segregation limit*. The interface between the constituent microdomains in strongly segregated systems is quite narrow (in the order of about 1 nm) with the monomer composition profile resembling a sharp step (fig 2.1b). In this regime the thermotropic order-order transitions (OOT) are not expected. The boundaries delineating the different microphases are expected to be vertical. The interaction energy associated with the A-B contacts is localised in the interfacial regions; the system would like to minimise the total area of such an interface by decreasing the energetically unfavourable contacts, but must do so under the constraint of incompressibility and entropic penalty of extended chain conformations. These opposing forces lead to perturbed chain configurations, and the periodicity L can be scaled as [11,14]: 6 / 1 3 / 2 χ aN R L∝ g ∝ (2.7)
Figure 2.1: Comparison of the one-dimensional composition profiles characterising a) WSL and b) SSL .
A wide variety of microstructure develops in block copolymer systems upon microphase separation (MS). The process of MS is a result of two competing effects. Firstly, dissimilar blocks prefer to segregate due to their inherent chemical incompatibility. The spatial extent of phase separation is, however, limited by the connectivity of the blocks imposed by the architecture of the molecules. As a compromise of both the effects, periodic microstructures evolve. The geometry of the microphase separated structure is, therefore, very sensitive to the chemical nature and molecular structure of the copolymer as well as its total composition. Unlike microphase separated block copolymers, the domain diameter in phase separated polymer blends are typically several hundred nanometers, and the morphology is independent of detailed features of the molecules .
Intermediate segregation regime (ISR) has also been reported in various block copolymers for 10.5 < χN < 29, where the domain periodicity scales as L ∝ N0.83e.g., for SB diblock, C. M. Papadakis, K. Almdal, K. Mortensen, D. Posselt: Identification of ISR in diblock copolymer systems, Europhys. Lett. 36, 289-294, (1996).
f r 2π/q* f r weak segregation strong segregation a) b)
Figure 2.2: Schematics of chain conformation at the microphase-separated state; a) stable flat interface from a compositionally symmetric AB block copolymer i.e. ΦA = ΦB, b) an unstable flat interface in the case ΦA >> ΦB and
c) a stable curved interface in the case of ΦA >> ΦB .
One of the most important factors determining the phase morphology in block copolymer is their composition. It is easily understood that the shape of the polymer/polymer interface varies with the relative chain length of the component polymer. A compositionally symmetric AB diblock copolymer (i.e., when volume fractions of both the components are the same) forms a flat interface as shown in figure 2.2 (a). As the volume fraction of a component continues to increase (say of A) relative to that of the other (i.e., as the copolymer becomes compositionally asymmetric) it is more likely that a curved interface is formed because the A chains must stretch sufficiently (fig 2.2b) to allow the formation of a planer interface. In this case the conformational entropy loss of the major component (here A) is too high. Therefore, the A chains tend to expand along the direction parallel to the interface to gain the conformational entropy under the condition that segment densities of both of the block chains have to be kept constant and must be the same as that of the bulk densities of the homopolymers. As a consequence the interface becomes convex towards the minor component (fig 2.2c). This effect of interface curvature becomes more and more pronounced as the composition of the block copolymer becomes further asymmetric. The morphological variations with composition observed in a two-component block copolymer are shown in fig 2.3 .
Figure 2.3: TEM images showing classical morphology of the block copolymers exemplified by that observed in an SI-diblock copolymer (A = PS and B = PI, the TEM images are from ref. .
The most asymmetric block copolymer possesses spherical morphology comprising body centred cubic (bcc) spheres of the minor component dispersed in the matrix of the major component. As the volume fraction of the minor component increases cylindrical morphology (hexagonal packed cylinders hpc of minor component in the matrix of major component) evolves.
Symmetric block copolymer exhibit a lamellar morphology consisting of alternating layers of the components. With increasing volume fraction of the component A the morphology appears in reversed order (i.e. hexagonal B cylinders in A matrix and A spheres in A matrix) [11,14]. In the strong segregation limit, the following sequence of phases is observed for PS/PI diblocks: fPS<0.17, bcc; 0.17< fPS <0.28, hex; 0.28< fPS <0.34, gyroid; 0.34< fPS <0.62, lam; 0.62< fPS
<0.66, gyroid; 0.66< fPS <0.77, hex; and 0.77< fPS, bcc .
The morphologies discussed above and illustrated in fig 2.3 are classical ones and are experimentally verified by different workers in several styrene/diene systems [16,17]. Recently, new non-classical bicontinuous morphologies have been found in SI diblock and star block copolymers and called ordered bicontinuous double diamond (OBDD) or ‘gyroid’ morphologies [18,19]. Hexagonal perforated layer structures (HPL), hexagonal modulated lamellar (HML) structures have been studied in various block copolymer systems both experimentally and theoretically (discussed by Hamley in ). Recent experimental results suggest that HML phase may be a transient, and the HPL a long-lived metastable phase. In contrast, gyroid morphology has been identified as one of the stable phases which consists of interpenetrating tetragonal network of the minor phase dispersed in three dimensionally continuous major phase matrix [18,19].
A number of unconventional morphologies were observed by Mogi et al. [20,21,22] and Hashimoto et al.  as well as Stadler and co-workers [24-26] and in ABC triblock copolymers which have opened new potential for controlling properties of these nanostructured materials. A few of these morphologies are cited in fig 2.4. Existence of a richer variety of morphology in ABC triblock copolymers is attributable to the presence of more interaction parameters (χAB,
χBC, χAC), and the morphological features are often complicated imposing difficulties in physical
interpretation [2,20-26]. These studies show that entirely different structures are formed in ABC triblock copolymers depending on the relative composition and interaction between the constituents. More complex morphologies have been recently predicted in three-component multi-block copolymers by Drolet and Fredrickson  and Bohbot-Raviv and Wang  using self consistent field (SCF) calculations which are yet to be experimentally confirmed. A few of these morphologies are indexed in Appendix 2.2.
2.2 Morphology Control via Architectural Modification
Development of living polymerisation techniques have enabled the chemists to design block copolymer molecules of well defined architectures. The block copolymer chains may range from simple two-component linear molecules to the multi-component radial and branched chains (star, miktoarm star, graft etc.). Most frequently studied important block copolymer architectures are schematically illustrated in figure 2.5. Various block copolymer architectures are dealt with in detail in recent monographs and reviews [2,29]. Architectural modification (modification of interface, chain topology, block symmetry etc.) may lead to a significant deviation in morphology and physical properties of the block copolymers. The strategies mainly adopted are briefly reviewed in the following paragraphs with special reference to two-component systems.
Figure 2.4: Scheme showing few newly discovered morphologies in three-component ABC triblock copolymers; a) tetragonal cylinder b) OTDD structure c) three-phase four-layer structure d) spheres between the lamellae and d) knitting pattern morphology; a-c are from Mogi et al. [20-22] and d-e are from Stadler et al. [25,26].
2.2.1 Variation of Chain Topology
This route consists of combining the block chains into different topologies: linear (diblock, triblock, multiblock), radial (simple star, miktoarm star), graft copolymers etc . Hadjichristidis and co-workers have synthesised a wide range of graft block copolymers, and studied their morphology formation and physical properties. Their works have been documented in recent articles and reviews [29-33]. A pronounced shift in phase behaviour of graft block copolymers with respect to corresponding diblock copolymers was observed. For example, lamellar morphology was observed in a PS/PI/PB miktoarm star block copolymer in a composition range in which a cylindrical morphology would be expected for a diblock copolymer having equivalent composition . The discrepancy in phase behaviour has been explained on the basis of packing frustration. Since both the elastomeric chains emanate from a common junction point in this particular star block copolymer, the chains tend to avoid chain stretching (and achieve maximum possible entropy) by relaxing and forming a curved interface [30-32]. Experimental
observation of ‘Mesh and strut’ structures by Hashimoto et al. , lamellae like structures (not exactly lamellae) by Yamaoka and Kimura  and of bicontinuous structures (later identified as Gyroid [18,19], in a composition range for cylindrical morphology in a linear block copolymer) by Thomas and co-workers in different star block copolymers are additional evidences illustrating the influence of block copolymer chain topology on their phase behaviour.
Figure 2.5: Block copolymers of various molecular architectures (A denotes the glassy block).
With the development of new synthetic methods, experimental studies on more complex architectures began to emerge, which, in turn, inspired new theoretical studies of the effect of molecular architecture on morphological behaviour. Milner calculated phase diagrams of asymmetric miktoarm star block copolymers and demonstrated that stability windows for a particular morphology is dramatically shifted as a function of block copolymer architecture . According to Milner’s theory, for example, lamellar morphology would be expected for a styrene/diene miktoarm star (A2B type) having styrene content as high as 81 vol %, for which
composition bcc spheres are expected in a diblock analogue. Particularly, the influence of asymmetry was analysed taking into consideration the molecular asymmetry parameter ε which constitutes both molecular architecture and conformational asymmetry. The theory has successfully predicted the phase behaviour of miktoarm star block copolymers and graft block copolymers.
The situation of morphology formation in an A2B type miktoarm star block copolymer is
schematically illustrated in fig 2.6 [30,32]. For a compositionally symmetric AB diblock (here named as (2A)B diblock), a flat interface is expected. If a trifunctional branching point (fig 2.6b) exists for A2B miktoarm star block copolymer, the A chains have to highly stretch perpendicular
to the interface in order to maintain the domain spacing constant. However, it is thermodynamically unfavourable, and the higher stretching of the two A arms can be partially alleviated by allowing the interface to curve away from them (fig 2.6c). Thus, multiple arms of block type A at a single junction result in an enhanced preference for these arms to remain on the convex side of the interface. This preference causes the shifts of order-order transition (OOT) lines towards higher B block volume fractions in morphology diagrams. The effect becomes more pronounced for a graft block copolymer (fig 2.6d).
Previously phase diagrams of asymmetric ABA triblock copolymers and star block copolymers was calculated by Dobrynin and Erukhimovich . These authors have shown the shift of phase boundaries with respect to the number of arms and symmetry of the arms of star block copolymers. Recent studies of Floudas  and Matsen and Schick  dealt also with phase diagrams of star block copolymers. Most recently, Morozov and Fraaije  have analysed the phase diagrams of the block copolymer melts with arbitrary architectures using the highly branched tree-like structures (dendrimers). Topology of the molecules was shown to considerably affect the spinodal temperature and asymmetry of the phase diagrams, but not their type and order.
2.6: Schematic of A-B junction points on an interface for a) (2A)B linear diblock copolymers, b) A2B block
copolymers with a trifunctional branch point at a flat interface, c) A2B single graft block copolymer with a
trifunctional branch point at a curved interface and d) A2B block copolymers with approximation of equal spacing
between the grafted A blocks. The curvature of the interface represents the shifts of the OOT lines towards higher B volume fractions on the morphology diagrams [30,32].
It should be mentioned that star block copolymers are earning special academic and technical interests due to their preferred rheological and mechanical properties [41-48]. Recently, Kennedy and co-workers have explored the synthesis of star block thermoplastic elastomers using living cationic polymerisation [45-48]. This group has intensively investigated the mechanical and rheological behaviour of linear and star block copolymers and shown that star copolymers possesses enhanced properties than their linear counterparts .
2.2.2 Asymmetric Block Structure
a) τ = 0.5 b) τ = 0.25
Figure 2. 7: Landau mean field phase diagram for an asymmetric ABA triblock copolymer with a) τ = 0.5 and b)
τ = 0.25 [49,51].
A1BA2 type copolymers having asymmetric block structure (where A and B are glassy and
rubbery blocks respectively; and MA1/MA2 ≠ 1) are of special technical importance. Highly
asymmetric A1BA2 block copolymers may combine the deformability of the shorter glassy end
blocks with strength of longer ones [42,52,53]. Asymmetry in block lengths is demonstrated to cause a significant morphological deviation both experimentally [31-33,41] and theoretically [36,37,39,49-51]. In ref. , it has been demonstrated that regions of phase stability in graft copolymers, asymmetric triblocks, linear multiblocks and poygraft copolymers are shifted with respect to diblock copolymer phase diagram. Mayes and Olvera de la Cruz [49,50] have extended Leibler’s theory to asymmetric triblocks and (AB)n star block copolymer melts and
generalised the influence of asymmetry as a reason for asymmetric phase diagram. They showed that the phase diagrams of ABA triblock copolymers (compositionally symmetric or asymmetric) are highly asymmetric. The composition (fc), at which the continuous transition from disordered
to lamellar phase occurs, was found to shift as a function of symmetry parameter. The points of continuous transition are also shifted in star block copolymers depending on the number of arms. Unlike in AB diblock copolymer, where a direct transition from disordered to lamellar phase occurs at f = 0.5, a transition from the disordered to hex and then to lam phase was predicted for a symmetric ABA triblock copolymer at this composition (asymmetric parameter, τ = NA1/NA1 +
disordered at f = 0.40 while it is predicted to have a hex phase at f = 0.60 (fig 2.7a). Meanwhile, for an asymmetric triblock copolymer, broad zones of bcc and hex stability are predicted (e.g., τ = 0.25, fig 2.7b).
The asymmetry of phase diagrams in an ABA triblock copolymer melts can be explained as follows: at fA = 0.40 (and fB = 0.60), it is entropically more difficult to confine two A blocks
into domains than a single B block, i.e., as the matrix component, the central B blocks must deform to accommodate the outer A blocks into A domains. Hence, the melt tends to be disordered. This problem is more notable for multiple arm stars with a core of connected B blocks. This causes the fc points to shift towards higher A volume fraction in (AB)n stars.
Recently, Matsen has examined the phase behaviour of asymmetric ABA triblock copolymer melt using self consistent field theory (SCFT) and pointed out that shift in phase transition lines results from their different segment distribution compared with that of symmetric triblocks as illustrated in fig 2.8 . As the value of τ deviates from 0.5 ( a AB diblock case), the A segment distribution moves away from the interface without stretching the A chains, and this causes an increase in domain spacing (fig 2.8b). Hence, the stretching energy in A domains is decreased. Further, the spontaneous curvature changes, since transferring some of the B domain stretching to the softer A domain by curving the interface away from B domains lowers the overall energy. This change in spontaneous curvatures shifts the OOTs toward larger fA as τ
decreases from 0.5, i.e., when the outer blocks become more asymmetric.
a) b) c)
Figure 2.8: Schematic diagram showing three triblock configurations all with equal degrees of chain stretching. A and B chains are represented by dotted and solid lines, respectively. a) symmetric triblock having its segments closest to the interface, b) asymmetric triblock with its segments away from the interface and c) asymmetric triblock having its shorter A block extracted from the A domains .
At sufficiently large asymmetry, the A chains begin to pull out of their domains. Although unfavourable interactions occur when A blocks leave A domains, it is more than compensated for by the fact that its B domains can relax. Figs 2.8b and 2.8c demonstrate how the extraction of A blocks allows the B segments shift away from the interface without further stretching of the molecule. The Extraction of short A blocks has a significant influence on the domain spacing of
the ordered morphologies. Generally, the domain periodicity is larger in asymmetric block copolymers than in equivalent symmetric triblocks and diblocks.
Furthermore, role of dispersity (e.g., polydispersity or even bidispersity as explained above) on the morphology formation was studied by Gerberding et al. using SBS triblock copolymers of variable molecular weight distribution of styrene and butadiene blocks . At a wide PS block molecular weight distribution, the bulk morphology was shifted to lower total volume fraction of polystyrene. Likewise, the morphology was shifted to lower PB content when the butadiene centre block possessed a wide molecular weight distribution.
2.2.3 Interfacial Modification
Introduction of a tapered or statistical chain between the incompatible blocks may further modify the block copolymer phase behaviour as demonstrated by several experimental [56-63] and a few analytical studies [64,65]. These studies have, in general, shown that presence of a tapered or statistical chain between the incompatible blocks results in a broadened interface due to enhanced mixing at the interface. In a systematic study, Gronski and co-workers [56,57] measured the thickness of interface in a series of styrene/diene copolymers as a function of length of tapered chain, and observed a broadened interfacial width (extended interface) with increasing length of the tapered chain. They have observed even three different phases in a two-component block copolymer system. Further interfacial modification in styrene/isoprene diblock copolymers was shown to change the interfacial tension (or the effective interaction parameter) and influence strongly the domain dimensions.
Zielinski and Spontak have modelled the equilibrium thermodynamics of A(A/B)B block copolymers (statistical or tapered middle block) by employing the confined chain statistics . Their model treats such systems as three component ABC block copolymers. In tapered block copolymers (fixed composition and molecular weight), the interfacial volume increased and domain periodicity decreased as the volume fraction of tapered block was increased. Both of these functional relationships suggests that a composition gradient imposed across the middle A/B block enhances the interfacial mixing. These predictions are in agreement with the findings of Gronski and co-workers [56,57].
However, microstructural characteristics of a series of compositionally symmetric tapered styrene/isoprene triblock copolymers investigated using TEM and SANS by Sameth et al. showed no dependence of domain periodicity with wt fraction of middle tapered block . Their study indicated, nevertheless, morphological deviations in A(A/B)B block copolymers having middle statistical or tapered block.
Recently, Knoll , Asai , Moctezuma and co-workers  have studied the influence of modified interface on the phase behaviour and mechanical properties of block copolymers. These
and similar studies  have indicated that the tapered transition may cause a significant increase in the effective volume fraction of the rubbery component and an improvement of ductility of the copolymers. In such block copolymers, the free energy component of the interface is sufficiently increased, and the system is driven towards order-disorder transition (ODT). Some block copolymer architectures having extended interface are schematically outlined in fig 2.9.
Figure 2.9: Block copolymers having broadened interface, a) inverse and b) normal tapered block copolymers  c) normal tapered triblock and d) triblock with a random A/B block ; white and black blocks represent glassy and rubbery chains, respectively.
Styrene/diene tapered block copolymers are intensively studied by Hashimoto and co-workers . THF was used as randomiser during the simultaneous copolymerization of styrene and diene using s-BuLi and benzene as initiator and solvent, respectively. They observed a rod-like morphology instead of lamellae in nearly symmetric copolymers. They have pointed out two phenomena that may be responsible for a shift in structural and thermomechanical properties of the block copolymers: domain boundary mixing (broadening of interface) and mixing in domain (incorporation of unlike segments into a particular domain).
Worm-like structures are observed by Knoll and Nießner in a highly asymmetric tapered SBS star block copolymer . More recently, Hadjichristidis and co-workers  have studied the phase behaviour of normal and inverse tapered block copolymers, and demonstrated that inverse tapered sequences lead to higher compatibility (wider interfacial width) than the normal ones. Further, the spinodal lines are shifted towards higher values of χN, which is in consistence with the theoretical predictions of Aksimentiev and Holyst . The latter authors have calculated the phase diagram of a gradient block copolymer melt using Landau-Ginzburg model, and predicted the stability of bcc, hex, gyroid and lam phases, similar to that of a diblock copolymer melt. However, the direct transition from disordered melt to lamellar phase was observed at χN = 11.906, in contrast to a value of 10.495 in a diblock copolymer. It has been mentioned that the ordering is caused at a larger characteristic length than in the diblock copolymer melt due to diffuse boundary between the blocks A and B.
Block copolymers possessing one or more of the variables discussed above (i.e. complex topology, asymmetric end blocks and broad interface) are expected to exhibit a complex phase behaviour which may have an important consequence on morphology formation, mechanical properties and deformation behaviour.
2.3 Blends Containing Block Copolymers 2.3.1 Block Copolymer/Homopolymer Blends
Block copolymers are often used in combination with other polymers or additives [52,62,68-70]. One of the important ways of morphology control in these materials is given by blending with homopolymers. A two component block copolymer may be blended with homopolymers which are identical with block copolymer’s constituent blocks or with homopolymers which are chemically different from that of the constituent homopolymers. Of particular industrial interests are the binary blends of styrene/butadiene block copolymers with polystyrene [52,68].
The length of the homopolymer chain compared to that of block copolymer primarily governs the phase behaviour of a binary blend of a block copolymer and a homopolymer. There is interplay between microphase and macrophase separation; and which effect predominates depends on the composition of the mixture [2,11,71-76]. Hashimoto et al. have explored the phase behaviour of binary blends consisting of styrene/diene copolymers and homopolymers by varying the molecular weight of homopolymer, composition of the blends, block copolymer architecture (AB diblock or ABA triblock) and by using homopolymers having different interaction with the block copolymer [71-76].
For styrenic block copolymer/homopolystyrene mixtures, three regimes have been identified depending on the degree of polymerisation of the homopolystyrene (NhPS) and that of the same
component of the block copolymer (NPS-block).
a. If NhPS < NPS-block, the hPS molecules tend to be selectively solubilized in the PS domain
of the microphase-separated copolymer, and is weakly segregated towards the domain centre leading to an increase in interfacial area per block and causing a swelling of the polystyrene block. This, in turn, can lead to a change in morphology (illustrated later in fig 2.11). This regime has been termed as ‘wet brush’ regime because the copolymer chains in the weak segregation regime can be considered to be polymeric brushes, and in this case they are ‘wetted’ by the penetration of homopolymer chains.
b. If NhPS ≈ NPS-block , the hPS is still selectively solubilized in the PS domains of the
microphase separated block copolymer. The hPS molecules tend to be localised in the middle of the PS domains. Hence, the interfacial area is not significantly affected, and the
conformations of another component chains are not significantly perturbed. In this ‘dry brush’ regime, PS block chains are not significantly swelled.
c. If NhPS > NPS-block, macrophase separation takes place leading to the formation of hPS
particles in the microphase-separated copolymer matrix or vice versa. Which component forms the matrix depends on the mixture composition.
Figure 2.10: a) Average interdomain distance L/Lo and b) average distance between the chemical junction a/ao
points alonmg the interface relative to that of pure PI diblock copolymer measured by SAXS with do = 26.7 nm and
ao = 2 nm in the regime MA-block > MhA .
Comprehensive studies on the phase behaviour of binary block copolymer/homopolymer blends was made by Hashimoto et al. [71-76] and Winey et al. [77,78]. Domain spacing and interfacial area per block were investigated in binary PS-PI block copolymer/PS blends using SAXS by Hashimoto and co-workers . For α ≤ 1 (where α is the ratio NhPS/NPS-block), the domain
spacing (L) and average distance between the junction points (a) were found to increase with increasing homopolymer concentration in the blends (fig 2.10). This suggests that the homopolymer chains have swelled the PS block domains. Furthermore, the magnitude of L increased with increasing α at given blend composition indicating the tendency of segregation of homopolymer chains towards the domain centre with increasingα.
Transitions from the lamellar phase of a neat PS-PI diblock copolymer to cylindrical and then to spherical structures were observed by Hashimoto [71,76] on addition of hPS. These morphological changes have been explained on the basis of changes in interfacial curvature and packing density as illustrated in fig 2.11. Addition of hPS chains causes the swelling of block PS chains of the copolymer leaving the PI blocks unswollen. This leads to a difference in segmental density in PS and PI phase. In order to retain normal liquid-like densities, the PS block must stretch and/or PI block must contract (fig 2.11b). However, an alternative is to curve the interface placing PS on its convex side (fig 2.11c). The latter situation predominates when the
conformational entropy loss due to chain stretching is overweighed by the interfacial curvature penalty.
Based on a series of experimental results on blends of styrene/diene diblock copolymers and hPS, Winey et al. have constructed a phase diagram at constant copolymer composition (about 50 vol %) by varying blend composition and α which show the region of existence of different phases which nearly correspond to that observed in pure block copolymers at corresponding overall composition. At larger value of α, homopolymer chains are completely expelled out of corresponding block domains which form a separate macrophase as shown by different studies [77,78].
Figure 2.11: Schematic illustration of chain packing: a) pure SI diblock copolymer chain with symmetrical volume fraction forming a flat interface, b) swelling of PS lamellae by uniform solubilization of hPS molecules causes stretching of PS-block chains and/or compression of PI-block chains resulting in a decrease in conformational entropy, c) alternatively a curved interface is formed to gain entropy .
Effect of copolymer architecture (star and triblock) on miscibility and mechanical properties of styrene/butadiene block copolymer/hPS was recently studied by Feng et al. [79-81]. These authors have suggested that there is a molecular weight range of hPS for which the mechanical properties are enhanced. Depending on the MhPS, added hPS was found to exist both in PS and
PB phases. The influence of block copolymer architecture on the miscibility of the blends was, however, not found.
In addition to classical phases, complex phases have been identified in block copolymer/homopolymer blends too [34,42,82]. Winey et al.  observed OBDD phase (later reassigned as ‘gyroid’ phase) in PS-PI diblock/hPS blends at a overall composition range ΦPS =
0.64-0.67 which is approximately same as the composition range in which this phase was observed in a pure PS-PI diblock copolymer (ΦPS = 0.62-0.66) . Hashimoto and co-workers
These structures and ‘catenoid lamellar structures’ reported by Disko et al.  resembled the HPL structures observed in diblock copolymer melts .
Low molecular weight hPS, though most soluble in the corresponding block domains of the block copolymers, is generally not desirable for technical applications. This, of course, may reduce the cost but also deteriorates the mechanical properties. Due to lack of stable entanglements, the products don’t possess optimum strength level. Therefore, hPS with quite higher molecular weights (∼ 100 kg/mole) is used. The molecular weight of hPS and PS block of the copolymer should be optimized since hPS tends to macrophase segregate when NhPS
approaches NPS-block, also undesirable because it may lead to loss in transparency.
Recently, Yamaoka has studied the morphology and toughness behavior of the blends of K-Resin 05 and a PS-co-PMMA (MS) using compression molded samples. His results show a macrophase separation of MS in K-Resin matrix [84,85]. Knoll and Nießner have studied the morphology and tensile properties of blends consisting of highly asymmetric star block copolymer and hPS using compression moulded samples . In spite of a large difference in the molecular weight of homopolystyrene and PS block of the block copolymer, no macrophase separation was observed. The star block copolymer was found to be especially compatible to the added homopolymer.
2.3.2 Binary Block Copolymer Blends
Compared to an intensive investigation of thermodynamics and phase behaviour of block copolymers, only limited information is available on their blends. Hoffman et al. investigated binary blends of SB diblocks and reported a microscopic demixing of blends, with two maxima in the domain size distribution . Jiang et al. , Hadziioannou et al.  and Hashimoto et al. [76,89,90] investigated binary blends consisting of diblocks and triblocks. In these studies, the blends were microphase separated; and depending on the blend composition and molecular weight of the copolymers, morphology transitions were also observed.
Studies of Hadziioannou et al. and Hashimoto et al. on a series of blends of lamellar diblocks and triblocks consisting of polystyrene and polyisoprene demonstrated that the phase behaviour of the binary block copolymer mixtures is mainly governed by copolymer composition, blend composition and molecular weight ratio (i.e M1/M2) of the copolymers [88-90]. If M1/M2 <5,
complete miscibility of the block copolymers was observed in which the domain periodicity followed the power law: L ~ Mn2/3, where Mn is the sum of mole fraction of each block
copolymer multiplied by corresponding number average molecular weight. When M1/M2 > 10,
only a partial miscibility of two lamellar block copolymers resulted in macrophase separation of lamellae having different lamellar periodicity . The morphology fundamentally different
from that of parent block copolymers was reported in blends of styrene/butadiene star block copolymers with nearly same chemical composition (ΦPS = 0.7) by Jiang et al. . Particularly,
coexistence of cylindrical and worm-like structures was observed. The molecular weight one of the star block copolymers was about 7 times higher than that of the other. The blends showed macrophase separated composite structures containing microphase separated composites. More recently, more complex structures are reported by Knoll and Nießner in blends of star block and triblock copolymers consisting of styrene and butadiene .
Recent investigations of Spontak et al. on the blends of symmetric (ΦPS = 0.5) and asymmetric
block copolymers (ΦPS = 0.85) showed that the blends show same microstructure as the pure
diblock having equivalent overall composition .
curved interface in a cylindrical diblock
segregation of short diblock to the interface
relieve of frustration by planer interface
Figure 2.12: Schematic illustrating packing frustration induced by addition of short diblock to a microphase of a long diblock .
It was shown that blending of a lamellar-forming diblock with ΦPS = 0.32 and one with ΦPS =
0.60 can induce the formation of bicontinuous cubic structure in certain ranges of composition. In contrast, blending of a diblock forming a lamellar phase with ΦPS = 0.44 with a diblock
forming a bicontinuous cubic structure with ΦPS = 0.66 resulted in the formation of lamellar
phase even when the overall composition was ΦPS = 0.62 (composition in which bicontinuous
structure is expected in a diblock) . It means that a single phase approximation cannot be used while considering the phase behaviour of blends of block copolymers having different molecular weights i.e., the blend morphology doesn’t necessarily reflect the morphology of a pure copolymer with an equivalent composition.
The morphology change may be induced by the interfacial curvature and packing density as schematically illustrated in fig 2.12 . Fig 2.12a shows a cylindrical block copolymer with B cylinders in the matrix of A. Exchanging one of the chains by a symmetric AB diblock (lamellae forming) leads to a situation shown in fig 2.12b. The segregation of a short diblock copolymer molecule to the interface leads to the low packing density (denoted by letter X in fig 2.12b where the copolymer is depleted leading to packing frustration). This frustration is relieved when the interface adopts a planer geometry which, in turn, leads to a transition from cylindrical to lamellar morphology (fig 2.12c).
More recently, Hashimoto et al. have studied the blends of AB diblocks with AC diblocks and reported the morphology as would be expected for ABC triblock copolymers . Abetz and Goldacker have reviewed morphology of ABC triblock copolymers and their blends, and shown the existence of hierarchies of microphase separated structures in binary ABC triblock copolymer blends . Through a systematic small angle neutron scattering (SANS) study of binary lamellar forming diblock copolymers, Papadakis et al. have constructed a phase diagram for such systems and demonstrated that a competition between microphase and macrophase separation takes place depending on the chain length ratio and composition [94,95].
These discussions reveal that research interests are growing in the study of phase behaviour of binary blends of block copolymers. These materials have, however, found no considerable industrial interest because of higher manufacturing costs of both the blend components. As a consequence, less (or almost no) attention has been paid in the deformation behaviour and mechanical properties of these blends.
2.4 Mechanical Properties and Deformation Behaviour
In the preceding section, morphology formation in block copolymers and the blends containing block copolymers is briefly reviewed. Now, a short review of micromechanical deformation processes observed in amorphous block copolymers as a function of microphase morphologies is presented. First the thermomechanical and mechanical properties of the polymeric materials are introduced.
2.4.1 Thermomechanical Properties
Figure 2.13: Dependence of complex modulus of elasticity as a function of temperature in different polymer pairs (schematic), case 1) immiscible polymers, 2) completely miscible polymers, 3) partially miscible polymers and 4) multitude of phases .
Mechanical properties of heterogeneous polymer systems are primarily determined by interaction between the phases and morphology resulting therefrom. Hence, analysis of miscibility of the components may provide an important insight into micromechanical and mechanical behaviour of heterogeneous systems including block copolymers.
Different spectroscopic and microscopic techniques, scattering methods and calorimetry can be employed to examine the miscibility and phase interaction in polymer pairs. However, the measurement of complex modulus as a function of temperature is the most important method for determining the miscibility of polymer mixtures. Four possible cases are schematically represented in fig 2.13 . Solid and broken lines stand for the mixture and pure components, respectively. Case 1 shows a solid curve indicating two distinct temperatures of glass transitions corresponding to those of the individual components A and B (broken lines). Here, two polymers are completely immiscible and are present as two separate phases. Amorphous two-component block copolymers generally belong to this class [43,69]. Case 2 shows a sharp glass transition roughly in between those of the two components. In this case, the polymers are completely miscible and exist as a single homogeneous phase. For example, a mixture of PMMA and PEO or PS and PPO represents this system . The curve in Case 3 indicates two separate glass transitions, but these are shifted with respect to the component homopolymers, i.e., both the phases are of mixed compositions. Weakly segregated block copolymers are known to form a partially miscible phase and hence exhibit a shift in glass transition temperature of constituents . Sometimes, three distinct phases may be observed in a two-component systems: two pure phases and a mixed phase as demonstrated by some block copolymers possessing broad interface [56,57]. Case 4 shows a broad, ill-defined glass transition reflecting the presence of a multitude of phases with a slightly different composition.
If the miscibility is desired, it can be realised by introducing a third ‘component’ to the binary polymer mixtures. Phase compatibiliser used in polymer blends, for example, enhance the miscibility (and hence phase adhesion) between the components. Of particular interest in the present work is to qualitatively analyse how the molecular architecture of the block copolymers influences their miscibility and phase behaviour.
2.4.2 Mechanical Behaviour of Polymers
Tensile experiments (stress-strain curves) offer a simple and straightforward way of characterising and comparing mechanical behaviour of polymeric materials. The total deformation of the test specimen comprises different material responses toward external stress: linear elastic, linear viscoelastic, non-linear viscoelastic and plastic deformation [1,8,98]. Linear elastic behaviour, which involves only the reversible alteration of inter-atomic distances without
breakage of chemical bond, is explained by the Hoock’s law. This region corresponds to less than 0.1% strain in thermoplastics. At higher strain (up to 0.5% strain), the deformation is no more linear elastic, and this region is termed as linear viscoelastic region, in which the strain-reversibility is time and temperature dependent. At strain >0.5%, the deformation is additionally a function of extent of loading besides time and temperature and called non-linear viscoelastic region. This region, where the molecular flow processes begin, follows the region of plastic deformation (stationary plastic flow) which finally leads to the specimen fracture. Depending on the phase morphology and micromechanical processes of deformation, mechanical behaviour observed in polymers can be classified as schematically summarised in figure 2.14 .
Figure 2.14: Characteristic stress-strain curves (schematic) of different polymers .
a) High modulus fibres (e.g., highly oriented fibres, reinforced thermoplastics): These materials are exclusively linear elastic. The stress increases linearly with strain leading to a high tensile strength a low elongation at break.
b) Brittle behaviour (e.g., unmodified PS, PMMA): The stress rises almost linearly with strain up to fracture. Stress increases slowly as the plastic deformation process like crazing onsets. The maximum strain is small (<10%).
c) Ductile behaviour (e.g., rubber modified thermoplastics, PVC): The stress increases with strain but drops after reaching the yield point. Macroscopic neck formation and stress whitening is observed.
d) Cold drawing (e.g., semicrystalline thermoplastics like PE, PP): The stress level remains practically constant after the strain softening (as observed in curve c in figure 2.14) when the neck expands over the whole specimen. The necking zone is stabilised by orientation hardening. This kind of behaviour is also found in some toughened thermoplastics like block copolymers.
e) Homogeneous deformation (e.g., TPEs, filled and unfilled rubbers): A slow and continuous increase in stress with strain is observed. The deformation is predominantly entropy elastic; yield points (if there are any) are diffuse.
Strain rate and test temperature have a strong influence on the mechanical properties of polymers (time temperature superposition principle [1,97,98]). Increasing strain rate and decreasing test temperature results in increasing tendency towards imbrittlement of samples which causes the mechanical behaviour of the polymers shift from right to left in fig 2.14. In ABA type block copolymers (where A and B are glassy and rubbery blocks, respectively), almost all the behaviours shown in fig 2.14 may be achieved by simply adjusting the copolymer composition at a temperature between Tg of both the components [43,68,69].
The mechanical behaviour of polymers outlined in fig 2.14 is closely associated with the underlying deformation mechanisms under given loading conditions. A sample which is brittle at a given test conditions may behave ductile under another set of conditions. Hence, the deformation mechanism changes from one test condition to the another. This behaviour is a consequence of pronounced viscoelastic property of the polymeric materials. The deformation mechanisms and resulting mechanical properties are further controlled by molecular and supramolecular parameters including nature of interface in the heterogeneous systems, dimension and organisation of the microscopic building blocks etc. [99-105]. Recently, unusual mechanical behaviours have been observed in the composites consisting of heterogeneous layers with dimensions in the range of few tens of nanometers [99,100]. The micromechanical behaviour of amorphous PS was found to differ considerably depending on molecular structure. In contrast to a linear PS which is characterised by the formation of fibrillated crazes under tension at room temperature, branched PS showed more ductile behaviour and homogeneous crazing under same set of conditions .
2.4.3 Micromechanical Construction of Polymers
Due to presence of a large variety of molecular and supramolecular structures, polymeric materials possess a wide variety of morphology. This makes it possible to modify their properties by altering one or more of these variables. How these variables finally lead to particular mechanical properties of polymeric materials is determined by the processes occurring in different length scales, from molecular to macroscopic level, as a response of the materials against external mechanical loading. These processes include displacement and scission of the chains, different yielding phenomena up to crack initiation, propagation and fracture [1,102,103]. These processes depend strongly on diverse molecular structures, morphology as well as loading conditions e.g., temperature, loading speed or stress state as already mentioned. Hence,
comprehensive knowledge of these micromechanical processes provides a direct way of designing polymeric materials with improved mechanical properties [103-105].
The fundamental deformation mechanisms observed in heterogeneous polymeric materials are discussed in [103,106]. Knowledge of these mechanisms is required to avoid the materials from undergoing premature failure, one of the main goals of polymer science and engineering. Inducing an intense plastic deformation over a large part of the sample and arresting the crack growth are generally useful to enhance toughness and strength of polymeric materials as schematically outlined in fig 2.15. A common idea of the toughening mechanisms outlined in fig 2.15A is to initiate a large number of local yielding zones (enhancing energy absorbing phenomena) which can be realised in the following ways :
a. Initiation of a number of microcracks by inorganic fillers, short fibers e.g.; CaCO3, glass
fibers, carbon fibers etc.
b. Incorporation of ductile fillers in brittle matrix which are stretched in the area of crack tip (bridging mechanism).
c. Inducing the formation of small local plastic zones (crazes or shear bands) which is induced by stress concentration at weak particles; a typical mechanism in rubber-toughened plastics.
d. Cavitation at or inside the filler particles, with subsequent stretching of the matrix ligament between the microvoids
Figure 2.15: Schematic representation of some general micromechanical mechanisms in heterogeneous polymers: A) mechanisms of enhancing the toughness and B) crack-stop mechanisms (cross-hatched areas are inorganic particles, fibres or weak particles dispersed in the bulk polymer matrix; σ stands for tensile stress) .